Standard Test Method for Corrosion of Surgical Instruments
NORMA vydaná dňa 1.2.2018
Označenie normy: ASTM F1089-18
Dátum vydania normy: 1.2.2018
Kód tovaru: NS-810362
Počet strán: 4
Približná hmotnosť: 12 g (0.03 libier)
Krajina: Americká technická norma
Kategória: Technické normy ASTM
boil test, copper sulfate test, corrosion tests, immersion test, surgical instruments,, ICS Number Code 11.040.30 (Surgical instruments and materials)
|Significance and Use|
3.1 This test method provides corrosion test methodologies and means of evaluation that serve as indicators of proper material selection and proper processing by the manufacturer.
Note 1: It is recommended that instruments be chemically passivated according to one of the treatments in Specification , electropolished according to Specification , or both, prior to evaluating the corrosion resistance according to this test method. The likelihood of failure may be higher for non-passivated instruments.
1.1 This test method covers general test procedures and evaluation criteria for the corrosion resistance of new and reusable surgical instruments fabricated from stainless steel alloys, such as, but not limited to, those listed in Specification .
1.2 Instruments containing stainless steel materials that are exclusive to the following shall use the boil test and the copper sulfate test: austenitic materials (Class 3), precipitation hardening materials (Class 5), and ferritic materials (Class 6) containing equal or greater than 16 % chromium.
1.3 Instruments containing any of the following stainless steel materials shall use the boil test: martensitic materials (Class 4) and ferritic materials (Class 6) containing less than 16 % chromium.
1.4 The copper sulfate test is used to detect the presence of free iron on the surface of materials.
1.5 The copper sulfate test as described in is not recommended for martensitic materials or for ferritic materials containing less than 16% chromium because these steels may give a positive indication irrespective of the presence or absence of anodic surface contaminants (see ).
1.6 The boil test is applicable to martensitic, austenitic, ferritic, and precipitation hardening materials to detect surface imperfections, free iron, or other anodic surface contaminants on stainless steel.
1.7 The values stated in SI units are to be regarded as standard. No other units of measurement are included in this standard.
1.8 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
1.9 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
|2. Referenced Documents|
Chcete mať istotu, že používate len platné technické normy?
Ponúkame Vám riešenie, ktoré Vám zaistí mesačný prehľad o aktuálnosti noriem, ktoré používate.
Chcete vedieť viac informácií ? Pozrite sa na túto stránku.
Posledná aktualizácia: 2018-10-20 (Počet položiek: 2 186 822)
© Copyright 2018 NORMSERVIS s.r.o.